advertisement

Analysis of Schottky Barrier Height in Small Contacts Using a Thermionic-Field Emission Model Moongyu Jang and Junghwan Lee This paper reports on estimating the Schottky barrier height of small contacts using a thermionic-field emission model. Our results indicate that the logarithmic plot of the current as a function of bias voltage across the Schottky diode gives a linear relationship, while the plot as a function of the total applied voltage across a metal-silicon contact gives a parabolic relationship. The Schottky barrier height is extracted from the slope of the linear line resulting from the logarithmic plot of current versus bias voltage across the Schottky diode. The result reveals that the barrier height decreases from 0.6 eV to 0.49 eV when the thickness of the barrier metal is increased from 500 Å to 900 Å. The extracted impurity concentration at the contact interface changes slightly with different Ti thicknesses with its maximum value at about 2.9×1020 cm-3, which agrees well with the results from secondary ion mass spectroscopy (SIMS) measurements. Manuscript received Dec. 14, 2001; revised June 28 and Aug. 8, 2002. Moongyu Jang (phone: +82-42-860-1896, e-mail: [email protected]) is with Basic Research Laboratory, ETRI, Daejeon, Korea. Junghwan Lee (e-mail: [email protected]) is with System IC R&D Division, HYNIX Semiconductor Inc., Cheongju, Korea. ETRI Journal, Volume 24, Number 6, December 2002 I. INTRODUCTION The contact between silicon and metal plays an important role in integrated circuit technology. The physics involved in this contact has been interpreted using the Schottky barrier concept. When the doping level in the silicon is low, the Schottky barrier acts as a diode that has a lower turn-on voltage than a p-n junction diode. With this advantage, the Schottky diode has been frequently used in high-speed devices such as those in GaAs [1], [2]. With an increased doping concentration at the interface, the Schottky diode becomes an ohmic contact with severe barrier lowering resulting from an increased tunneling current [3], [4]. Many experimental and theoretical studies of the current flow mechanism in Schottky barriers have been reported [1][10]. Crowell and Sze used Schottky’s diffusion theory and Bethe’s thermionic emission theory to evaluate the Schottky barrier [5]. They included the effects of image force rounding of the barrier and the potential transition from image force to conduction band in the metal. Padovani and Stratton analyzed tunneling currents in Schottky barriers from the standpoint of field and thermionic-field emission using a one dimensional Wentzel-Kramer-Brillouin (WKB) approximation [7]. However, their analysis ignored image force effects and used a simple parabolic barrier shape. The WKB approximation is valid only for smoothly varying potential profiles and, therefore, is not accurate at the top of the barrier [5]. Recently, Sassen, Witzigmann, Wolk, and Brugger analyzed a Schottky diode using the transfer matrix method in GaAs. Their result was expressed as an integral including the transmission coefficient T, which requires numerical analysis [1]. Shenai and Moongyu Jang et al. 455 Dutton analyzed a Schottky barrier using image force effects, surface charge density, and the dipole effect, which was modeled as a single exponential decay of the total interface charge. They also considered the series resistance in a Schottky barrier device [2]. The thermionic emission theory applies when the barrier height is much larger than the thermal energy and the current flow depends mainly on the barrier height. In this case, the logarithmic plot of the current with applied voltage gives a linear line, and thus allows easy analysis of the barrier height and ideality factor. However, as the impurity concentration increases, thermionic-field emission becomes the dominant factor and the current flow depends on both the barrier height and the impurity concentration. In thermionic-field emission, the logarithmic plot of the current with applied voltage deviates from a linear behavior as the tunneling current increases. Note that it is difficult to extract Schottky barrier energy and impurity concentration since the plot is not linear. To investigate the characteristics of the Schottky diode, three methods—current-voltage measurement, activation energy measurement, and photoelectric measurement—have been widely used [8]. However, for the very small contacts used in deep submicron technology, it is difficult to use activation energy measurement and photoelectric measurement due to area restriction. Therefore, current-voltage measurement is the best method for very small contacts. In deep submicron metal contacts, the thickness of the barrier metal plays a critical role in contact resistance and leakage current. The Ti/TiN stack layer has been widely used as a barrier metal [11]. However, the Ti thickness is a major factor in the contact resistance since it reacts with silicon, and thus forms TiSi2. The reaction rate between Ti and Si depends on the Ti thickness and doping concentration in the junction. It is not well understood how the Schottky barrier behaves with different Ti thicknesses in a small contact. In this work, the Schottky barriers of small metalsemiconductor contacts as a function of Ti thickness are estimated using the thermionic-field emission model based on the forward biased current-voltage measurement method. II. THEORY The four mechanisms by which carrier transport occurs in Schottky barriers are thermionic emission over the potential barrier, carrier tunneling through the potential barrier, carrier recombination and/or generation in the depletion region, and carrier recombination in the neutral region, which is equivalent to minority-carrier injection. In these mechanisms, the dominant modes of carrier flow in metal-semiconductor 456 Moongyu Jang et al. contacts are thermionic emission and carrier tunneling [9]. In an ideal metal-semiconductor system, the potential energy barrier to the flow of charge carriers is primarily determined by the work-function difference between the metal and the semiconductor. In practice, however, the barrier height also varies as a function of electric field and impurity concentration at the interface. Padovani and Stratton assumed a simple parabolic barrier shape by ignoring barrier lowering due to image force and uniform doping. In an intermediate temperature range, where thermionic-field emission is dominant, the current density in the forward direction is expressed by the following equation [7]. J = J S exp(qV / E00 ). (1) Ignoring the error function term [7], the saturation current is given as JS = Aπ 1/ 2 E001/ 2 ( EB − qV + ξ 2 )1/ 2 kT cosh( E00 / kT ) ξ 2 EB + ξ 2 exp − E00 kT , (2) where EB is the potential energy of the top of the barrier with respect to the Fermi level of the metal, V is the applied bias between the metal and the semiconductor, ξ2 is the energy of the Fermi level of the semiconductor measured with respect to the bottom of its conduction band, k is the Boltzmann constant, T is the Kelvin temperature, and A is the classical Richardson constant. E00 is a constant related to the WKB expression for the transmission of the barrier and is given as follows [6]. E00 = 1.85 ×10 −11 ( N / mr ⋅ εr ) 1/ 2 eV, (3) where N is the doping concentration at the metalsemiconductor interface in the unit of cm-3, mr is the tunneling effective mass measured in the unit of the free electron mass, and εr is the relative dielectric constant of silicon. If the externally applied voltage across the metalsemiconductor is much smaller than the Schottky barrier (i.e., qV≪EB), the voltage dependency of the saturation current JS can be ignored and the current density can be expressed as follows. J = J S 0 exp(qV / E00 ), J SO = Aπ 1/ 2 E001/ 2 ( EB + ξ 2 ) 1/ 2 kT cosh( E00 /kT ) ξ 2 EB + ξ 2 exp − E00 kT (4) , (5) ETRI Journal, Volume 24, Number 6, December 2002 where JS0 is the saturation current without applied voltage. Note that the logarithmic plot of the current density as a function of the applied bias V gives a straight line of slope q/E00, and from the extracted E00, the impurity concentration can be calculated by (3). Also, the Schottky barrier height EB can be calculated using (5). The specific contact resistance Rc, which is an important factor in ohmic contacts, is defined by the following equation [2], [4]. −1 E00 ∂J . RC ≡ = ∂V V = 0 q ⋅ J S 0 (6) By replacing E00 with kT, the expression of Rc in (6) becomes comparable to the result from the thermionic emission model [8]. respectively. The current-voltage curve is measured in a CBKR pattern to exclude parasitic resistance components. As the figure shows, the measured log I-V curve is not linear. Sze asserted that if thermionic emission is dominant, which is the major current flow mechanism for low impurity concentrations, the curve should be linear [8]. Padovani and Stratton reported that even if thermionic-field emission is dominant, which occurs at a highly doped metalsemiconductor interface, the log I-V curve is approximately linear with applied bias voltage [7], while Lepselter and Andrews wrote that if direct tunneling is dominant, the current is directly proportional to the applied bias [10], which implies the ideal ohmic contact. However, our result in Fig.1 indicates that the I-V characteristics of the contact do not follow the behavior of any of these three models. III. EXPERIMENTAL IV. RESULTS AND DISCUSSION Figure 1 shows the logarithmic current-voltage (I-V) plot of the manufactured metal-semiconductor contact: closed circles, open squares, and closed diamonds correspond to measured data with Ti thicknesses of 500 Å, 700 Å, and 900 Å, ETRI Journal, Volume 24, Number 6, December 2002 1E6 J (A/cm2) We used a 0.25 µm embedded DRAM process to fabricate the metal contact to the p+ junction in N-Well using a p-type <100> silicon substrate with resistivity from 9 to 12 Ω-cm. After formation of the modified LOCOS isolation and gate patterning, a p+ junction was formed by BF2 implantation with an energy level of 30 keV and a dose of 2.0 × 1015 cm2. After forming the DRAM cell, we used a CMP process for planarization. After patterning the metal contact by deep UV lithography, we used dry etching to open the contact holes. The metal contact depth was 2.4 µm and the size 0.32 µm × 0.32 µm. Note that the DRAM cell topology caused the deep metal contact. After removing the native oxide in the contact hole using a buffered oxide etchant, we deposited a barrier metal and annealed it at 650 °C for 10 min to form TiSi2 at the metalsemiconductor interface. To investigate the variation of the Schottky barrier’s height according to the thickness of the barrier metal, we chose thicknesses for the Ti: 500 Å, 700 Å and 900 Å. We filled the contact hole with tungsten and used aluminum for the metal line. The contact resistance was measured by the Cross Bridged Kelvin Resistor (CBKR) pattern and the current-voltage characteristics of the contact by a semiconductor parameter analyzer (HP4156A). We investigated the interface morphology between the barrier metal and the silicon junction using transmission electron microscopy (TEM). 1E7 Ti = 500Å Ti = 700Å 1E5 Ti = 900Å 1E4 0 0.2 0.4 0.6 0.8 1 VTOT (V) Fig. 1. I-V characteristic curve of the metal-semiconductor contact in a highly doped p+ junction. The contact hole size is 0.32 µm×0.32 µm. Closed circles, open squares, and closed diamonds represent data with Ti thicknesses of 500 Å, 700 Å, and 900 Å, respectively. Figure 2 shows the voltage dependence of the contact resistance. The components of the contact resistance can be divided into two parts: the Schottky diode and the spreading resistance caused by current crowding that is due to the small size of the contact. The non-linear behavior depicted in Fig. 1 is caused by spreading resistance, which is negligible in relatively larger contacts. In Fig. 2, the resistance approaches 220 Ω, irrespective of the thickness of the barrier metal, as the applied bias voltage increases. This is likely related to current crowding in a small contact hole as reported in [2] and [11]. As mentioned, the total resistance across the contact consists of Rdi caused by the Schottky diode and Rsp caused by spreading resistance as the Moongyu Jang et al. 457 inserted equivalent circuit in Fig. 2 explains. Note that Rdi depends on the applied voltage, while Rsp depends not on applied voltage, but on contact size and doping level. Hence, as the voltage difference between the VH and VL nodes increases, Rdi approaches zero because of the increased thermionic-field emission and the total resistance is identical to Rsp. Therefore, from the results of Fig. 2, we can deduce that Rsp is 220 Ω. The closed and open circles correspond to the voltage applied across the Schottky diode (Vdi) and the spreading resistor (Vsp), respectively. It appears that Vdi saturates at 0.375 V, while Vsp increases linearly as the total applied bias increases. The figure shows clearly that the ohmic characteristic is achieved when the applied voltage between the VH and VL node exceeds 0.75 V. (a) Contact resistance (×10-6Ωcm2) 4 Plugged W Ti = 500Å Ti = 700Å Ti = 900Å 3 VH Rdi Vi 2 Rsp Ti-Silicide VL 1 90.00 nm (b) 0 0 0.2 0.4 0.6 0.8 1 Plugged W VTOT (V) Fig. 2. The variation of contact resistance with applied bias across the Kelvin resistor. The contact hole size is 0.32 µm × 0.32 µm. Closed circles, open squares, and closed diamonds represent data with Ti thicknesses 500 Å, 700 Å, and 900Å, respectively. The insert represents the equivalent circuit of the resistor in a CBKR pattern assuming that the Schottky diode and spreading resistor is serially connected. Rdi denotes the resistance of the Schottky diode and Rsp denotes the spreading resistance. VH-VL corresponds to the externally applied bias voltage across the Kelvin resistor and Vi represents the voltage between the Schottky diode and spreading resistor. The effect of barrier metal thickness is clearly shown in Fig. 2. The specific contact resistance, which is the contact resistance at zero bias voltage, increases abruptly at a Ti thickness of 500 Å. This is probably because not enough TiSi2 formed at the interface due to the very deep contact height and small contact size, which resulted in an increase of the Schottky barrier height at a Ti thickness of 500 Å. In fact, the TEM images of the contacts with different Ti thicknesses clearly show that the TiSi2 layer formed with a Ti thickness of 500 Å is not uniform and has a relatively much thinner TiSi2 layer in some parts (Fig. 3). Note that the formed TiSi2 layers are very uniform when the Ti thickness exceeds 700 Å. Figure 4 shows the dependency of the voltage drop across the Schottky diode (Vdi) and spreading resistance (Vsp) as a function of the applied voltage for a Ti thickness of 500 Å. 458 Moongyu Jang et al. Ti-Silicide 90.00 nm (c) Plugged W Ti-Silicide 90.00 nm Fig. 3. TEM images of metal-semiconductor interface. (a), (b), and (c) represent images with thicknesses 500 Å, 700 Å, and 900 Å, respectively. ETRI Journal, Volume 24, Number 6, December 2002 Vdi and Vsp (V) 1.2 Ti thickness : 500Å 0.9 0.6 0.375V 0.3 0 0 0.5 1 1.5 2 VH-VL (V) Fig. 4. The voltage components in CBKR for 500 Å Ti. Closed and open circles represent the voltage component biased across the Schottky diode (Vdi) and spreading resistor (Vsp), respectively. To accurately analyze the thermionic-field emission model, the net applied voltage across the Schottky diode (Vdi) should be used instead of the total applied bias across the CBKR pattern (VH-VL), since the CBKR pattern does not give a linear relationship in the logarithmic plot of the current to the total applied voltage, as discussed in relation to Fig. 1. Figure 5 shows the logarithmic plot of the current as a function of Vdi at different Ti thicknesses. Closed circles, open squares, and closed diamonds represent the measured data for Ti thicknesses of 500, 700, and 900 Å, respectively. It appears that the plots in Fig. 5 are linear, while the logarithmic plot of the current as a function of the total applied voltage deviates from the linear line as shown in Fig. 1. We used the least square fitting method for straight lines to extract E00 and JS0. The logarithmic linear dependency of the current on the net bias voltage across the Schottky diode (Vdi) strongly supports the validity of our assumption of voltage dependency in JS and the use of (5). In Fig. 5, E00 is calculated from the slope, while JS0 is obtained from the intersection of the Y-axis. With the extracted E00 and JS0, the impurity concentration N, Schottky barrier height EB, and specific contact resistance Rc are calculated by applying (3), (5), and (6), respectively. Table 1 summarizes the extracted parameters. In the calculation of the Schottky barrier height EB and impurity concentration N, the effective tunneling mass (mr) for the hole, the Richardson constant (A) for the <100> p-type substrate, and ETRI Journal, Volume 24, Number 6, December 2002 the relative dielectric constant (εr) are assumed as 0.9163, 79 Acm-2 K-2, and 12, respectively [4], [12], [14]. It appears that the extracted Schottky barrier height decreases from 0.60 eV to 0.49 eV when the Ti thickness increases from 500 Å to 900 Å. The higher Schottky barrier height for the 500 Å Ti thickness may come from the imperfect formation of TiSi2 deduced from the irregular interface morphology in Fig. 3. Typically, in a low doped Schottky diode, the barrier height of p+ is about 0.70 eV [8]. However, the barrier height is lowered in a highly doped p+ junction due to the image charge and tunneling. If the impurity concentration is 1020 cm-3, the calculated depletion width is about 28 Å and the barrier lowering by the image charge is 0.225 eV [2], [8]. When the barrier lowering in a highly doped p+ junction is considered, the extracted Schottky barrier height is comparable to the results of previous work [8], [13]. Table 1 reveals that the extracted maximum concentration of impurity is about 2.9 × 1020 cm-3, which is comparable to our secondary ion mass spectroscopy (SIMS) result (Fig. 6). 15 14 ln J = 11.20Vdi + 11.27 13 ln J = 10.97Vdi + 10.92 ln J (A/cm2) 1.5 12 11 ln J = 13.03Vdi +9.11 10 9 0 0.1 0.2 0.3 Vdi (V) Fig. 5. The logarithmic plot of current with net bias voltage applied across the Schottky diode (Vdi). Closed circles, open squares, and closed diamonds represent data with Ti thicknesses of 500 Å, 700 Å, and 900Å, respectively. Table 1. Summary of extracted parameters. Ti thickness [Å] E00 [eV] JS0 [A-cm-2] Rc [Ω-cm2] N [cm-3] EB [eV] 500 0.0767 9.08E3 5.09E-6 2.06E20 0.60 700 0.0911 5.51E4 9.98E-7 2.91E20 0.53 900 0.0893 7.83E4 6.83E-7 2.80E20 0.49 Moongyu Jang et al. 459 0.7 1E21 Boron Phosphorus 0.5 EB (eV) B, F, P Concen. (atoms/cm3) 0.6 Fluorine 1E20 1E19 0.3 0.16 µm 1E18 0.4 0.2 0 1E17 1 2 3 107/Ti Thickness (Å-1) 1E16 0.00 0.05 0.10 0.15 0.20 0.25 0.30 Depth (µm) Fig. 8. The dependence of Schottky barrier height to Ti thickness, which clearly shows an inversely proportional characteristic. From this graph, the minimum achievable Schottky barrier height can be estimated with Ti thickness. Fig. 6. The SIMS profile of the p+ junction. Figure 7 shows the logarithmic plot of specific contact resistance (Rc) versus EB /sqrt(N), which validates the analysis in this work. In the region dominated by thermionic-field emission and direct tunneling, the variation of the logarithmic specific contact resistance with EB/sqrt(N) should be linear as shown in [3], [8]. The linear variation indicates that the major current flow mechanism is thermionic-field emission. The figure also indicates that the specific contact resistance can be reduced by up to 10% if the barrier height and impurity concentration are optimized. Figure 8 shows the variation of the Schottky barrier as a function of Ti thickness. As shown, the Schottky barrier is inversely proportional to the Ti thickness. Note that the minimum barrier height is 0.33 eV with unlimited Ti thickness. -4 -5 log (Rc) -6 -7 -8 V. CONCLUSION We used current-voltage measurements to extract the Schottky barrier height of small contacts. The metalsemiconductor contact in a highly doped junction shows nonideal diode curves, which is caused by spreading resistance. Therefore, we extracted the net applied bias voltage across the Schottky diode by assuming a serial connection between the Schottky diode and the spreading resistor. It appears that when the net bias voltage is applied across the Schottky diode, the I-V curves follow the thermionic-field emission model. Using this model, we extracted the Schottky barrier height and impurity concentration. Our investigation revealed that the barrier height decreased from 0.6 eV to 0.49 eV when the thickness of the barrier metal was increased from 500 Å to 900 Å. The extracted impurity concentration at the contact interface changed slightly with a changing Ti thickness with its maximum value at about 2.9 × 1020 cm-3, which is in good agreement with the result from our SIMS measurement. REFERENCES -9 0 0.1 0.2 0.3 0.4 0.5 1010×EB/Sqrt (N) Fig. 7. The log(Rc) versus EB/sqrt(N) graph. In thermionic-field emission and direct tunneling dominant region, the graph shows linear behavior. 460 However, the junction leakage current increases as the barrier metal thickness increases because of excessive Ti atoms. From our experiments, 900 Å of Ti is optimal in terms of contact resistance and junction leakage. Moongyu Jang et al. [1] Stefan Sassen, Bernd Witzigmann, Claus Wolk, and Hans Brugger, “Barrier Height Engineering on GaAs THz Schottky Diodes by Means of High-Low Doping, InGaAs- and InGaPLayers,” IEEE Trans. Electron Devices, vol. 47, 2000, pp. 24-32. [2] Krishna Shenai and Robert W. Dutton, “Current Transport ETRI Journal, Volume 24, Number 6, December 2002 Mechanisms in Atomically Abrupt Metal-Semiconductor Interfaces,” IEEE Trans. Electron Devices, vol. 35, 1988, pp. 468482. [3] A.Y.C. Yu, “Electron Tunneling and Contact Resistance of MetalSemiconductor Contact Barriers,” Solid-State Electronics, vol. 13, 1970, pp. 239-247. [4] C.Y. Chang, Y.K. Fang, and S.M. Sze, “Specific Contact Resistance of Metal-Semiconductor Barriers,” Solid-State Electronics, vol. 14, 1971, pp. 541-550. [5] C.R. Crowell and S.M. Sze, “Current Transport in MetalSemiconductor Barriers,” Solid-State Electronics, vol. 9, 1966, pp. 1035-1048. [6] C.R. Crowell and V.L. Rideout, “Normalized Thermionic-Field (T-F) Emission in Metal-Semiconductor (Schottky) Barriers,” Solid-State Electronics, vol. 12, 1969, pp. 89-105. [7] F.A. Padovani and R. Stratton, “Field and Thermionic-Field Emission in Schottky Barriers,” Solid-State Electronics, vol. 9, 1966, pp. 695-707. [8] S.M. Sze, Physics of Semiconductor Devices, 2nd ed., New York, Wiley, 1981. [9] M.S. Tyagi, Physics of Schottky Barrier Junctions in Metal Semiconductor Schottky Barrier Junctions and Their Applications, B.L. Sharma, ed., New York, Plenum, 1984, pp. 1-60. [10] M.P. Lepselter and J.M. Andrews, “Ohmic Contacts to Silicon,” The Electrochemical Society Symposium Series, New York, 1969, pp. 159-186. [11] S. Wolf, Silicon Processing for the VLSI Era, LATTICE PRESS, 1990. [12] H.D. Barber, “Effective Mass and Intrinsic Concentration in Silicon,” Solid-State Electronics, vol. 10, 1967, pp. 1039-1051. [13] Krishna Shenai, “Effect of Arsenic Implantation on Electrical Characteristics of LPCVD WSi2/n-Si Schottky Contacts,” IEEE Trans. Electron Devices, vol. 38, 1991, pp.2033-2035. [14] C.R. Crowell, “Richardson Constant and Tunneling Effective Mass for Thermionic and Thermionic-Field Emission in Schottky Barrier Diodes,” Solid-State Electronics, vol. 12, 1969, pp. 55-59. ETRI Journal, Volume 24, Number 6, December 2002 Moongyu Jang was born in Korea on October 18, 1968. He received the BS degree in physics at Kyungpook National University, Daegu, Korea, in 1991 and the MS degree and PhD degree in physics at Korea Advanced Institute of Science and Technology (KAIST), Daejeon, Korea, in 1993 and 1997. In 1997, he joined HYUNDAI Electronics Inc., Ichon-Si, Korea (Now HYNIX Semiconductor Inc.), where he was involved in the process integration of MDL (Merged DRAM and Logic) devices. From 1997 to 1998, he was involved in the development of 0.35 µm MDL technology. From 1999 to 2001, he was involved in the development of 0.18 µm MDL technology. Now he has moved to Electronics and Telecommunications Research Institute (ETRI), Daejeon, Korea, where he is involved in the basic research on nano MOSFET devices. His research interests include process integration and analysis of nano scale MOSFET and Schottky barrier tunnel transistors (SBTT), and mesoscopic quantum transport phenomena. Junghwan Lee received the PhD degree in chemical engineering from Drexel University, Philadelphia, in 1996, the MS degree from Korea Advanced Institute of Science and Technology, Seoul, Korea, in 1985, and the BS degree from Hanyang University, Seoul, Korea, in 1983. In 1985, he joined Samsung Electronics Company, Ltd., Gyeonggi-do, Korea, where he was involved in development of 64 Kb, 256 Kb, and 1 M SRAMs as a process integration engineer. In 1989, he joined Hyundai Electronics Industries Co. Ltd. where he was engaged in development of 4 M, 16 M, and 64 M DRAMs as a process integration manager. He rejoined Hyundai Electronics in 1996 and led a device group for development of 0.13 µm DRAM technology. In 1997, he moved to MML (Merged Memory/Logic) device group and has managed the development of 0.35 µm, 0.25 µm, and 0.18 µm MML technology. His current interests are MML device of beyond 0.15 µm and merged Ferroelectric technology as well as yield-up of MML products. Moongyu Jang et al. 461